Presentation on theme: "Chem 754 - Solid State Chemistry Ionic Conductivity and Solid Electrolytes I: The Basics Chemistry 754 Solid State Chemistry Lecture #26 June 2, 2003."— Presentation transcript:
Chem Solid State Chemistry Ionic Conductivity and Solid Electrolytes I: The Basics Chemistry 754 Solid State Chemistry Lecture #26 June 2, 2003
Chem Solid State Chemistry References A.R. West – “Solid State Chemistry and it’s Applications”, Chapter 13, Wiley (1984) C.N.R Rao and J. Gopalakrishnan – “New Directions in Solid State Chemistry”, pp , Cambridge (1997) A. Manthiram & J. Kim – “Low Temperature Synthesis of Insertion Oxides for Lithium Batteries”, Chem. Mater. 10, (1998). J.C. Boivin & G. Mairesse – “Recent Material Developments in Fast Oxide Ion Conductors”, Chem. Mater. 10, (1998). Craig Fisher (Japan Fine Ceramic Institute)
Chem Solid State Chemistry Solid Electrolytes Electrolyte - A substance that conducts electricity through the movement of ions. Most electrolytes are solutions or molten salts, but some electrolytes are solids and some of those are crystalline solids. Different names are given to such materials: –Solid Electrolyte –Fast Ion Conductor –Superionic Conductor Over the next two lectures we will be looking at materials which behave as solid electrolytes, their properties and applications.
Chem Solid State Chemistry Ionic vs. Electronic Conductivity Let’s begin by comparing the properties of ionic conductors with the conventional electronic conductivity of metals. Metals –Conductivity Range = 10 S/cm < < 10 5 S/cm –Electrons carry the current –Conductivity Increases linearly as temperature decreases (phonon scattering decreases as T ) Solid Electrolytes –Conductivity Range = S/cm < < 10 S/cm –Ions carry the current –Conductivity decreases exponentially as temperature decreases (activated transport)
Chem Solid State Chemistry Defects In order for an ion to move through a crystal it must hop from an occupied site to a vacant site. Thus ionic conductivity can only occur if defects are present. The two simplest types of point defects are Schottky and Frenkel defects. Schottky Defect (i.e. NaCl) Na + + Cl - V na + V Cl Frenkel Defect (i.e. AgCl) Ag + V Ag + Ag + interstitial
Chem Solid State Chemistry Ion Migration (Schottky Defects) Consider the movement of Na + ions in NaCl via vacancies originating from Schottky defects. Note that the Na + ion must squeeze through the lattice, inducing significant local distortion/relaxation. This is one factor that limits the mobility of ions. A second factor that contributes is the relatively high probability that the ion will jump back to it’s original position, leading to no net ionic migration. To get across the unit cell into the vacancy the Na + ion must hop through the center of the cube where it squeezes by 4 Cl - and 2 Na +. The energy of this “transition state” will determine the ease of migration. Na NaNaCl Cl ClCl E
Chem Solid State Chemistry Ion Migration (Frenkel Defects) The Frenkel defects in AgCl can migrate via two mechanisms. Ag AgAgCl Cl ClCl Ag 2 Ag 1 AgAg Cl Cl Ag AgAgCl Cl ClCl Ag 2 Ag 1 AgAg Cl Cl Ag AgAgCl Cl ClCl Ag 2 AgAg Cl Cl Ag AgAgCl Cl ClCl Ag 1 AgAg Cl Cl Direct Interstitial Jump Interstitialcy Mechanism
Chem Solid State Chemistry Applications of Ionic Conductors There are numerous practical applications, all based on electochemical cells, where ionic conductivity is needed and it is advantageous/necessary to use solids for all components. –Batteries –Fuel Cells –Gas Sensors In such cells ionic conductors are needed for either the electrodes, the electrolyte or both. –Electrolyte (Material needs to be an electrical insulator to prevent short circuit) –Electrode (Mixed ionic and electronic conductivity is needed to avoid open circuit) Electrolyte Anode Cathode Useful Power e -
Chem Solid State Chemistry Schematic of a Solid Oxide Fuel Cell Taken from
Chem Solid State Chemistry Schematic of Rechargable Li Battery Taken from A. Manthiram & J. Kim – “Low Temperature Synthesis of Insertion Oxides for Lithium Batteries”, Chem. Mater. 10, (1998).
Chem Solid State Chemistry Solid Electrolyte Materials Ag + Ion ConductorsAg + Ion Conductors –AgI & RbAg 4 I 5 Na + Ion ConductorsNa + Ion Conductors –Sodium -Alumina (i.e. NaAl 11 O 17, Na 2 Al 16 O 25 ) –NASICON (Na 3 Zr 2 PSi 2 O 12 ) Li + Ion ConductorsLi + Ion Conductors –LiCoO 2, LiNiO 2 –LiMnO 2 O 2- Ion ConductorsO 2- Ion Conductors –Cubic stabilized ZrO 2 (Y x Zr 1-x O 2-x/2, Ca x Zr 1-x O 2-x ) – -Bi 2 O 3 –Defect Perovskites (Ba 2 In 2 O 5, La 1-x Ca x MnO 3-y, …) F - Ion ConductorsF - Ion Conductors –PbF 2 & AF 2 (A = Ba, Sr, Ca)
Chem Solid State Chemistry -AgI & RbAg 4 I 5 have ionic conductivities comparable to conc. H 2 SO 4 Stabilized ZrO 2 is not a good ionic conductor at low temperature. Taken from “Solid State Chemistry and it’s Applications” by Anthony West
Chem Solid State Chemistry General Characteristics: Solid Electrolytes 1.A large number of the ions of one species should be mobile. This requires a large number of empty sites, either vacancies or accessible interstitial sites. –Empty sites are needed for ions to move through the lattice. 2.The empty and occupied sites should have similar potential energies with a low activation energy barrier for jumping between neighboring sites. –High activation energy decreases carrier mobility, very stable sites (deep potential energy wells) lead to carrier localization. 3.The structure should have solid framework, preferable 3D, permeated by open channels. –The migrating ion lattice should be “molten”, so that a solid framework of the other ions is needed in order to prevent the entire material from melting. 4.The framework ions (usually anions) should be highly polarizable. –Such ions can deform to stabilize transition state geometries of the migrating ion through covalent interactions.
Chem Solid State Chemistry Molten Sublattice (1/2 Melting) In the best ionic conductors one ion becomes so mobile that for all intensive purposes those ions are in a “molten” state. This behavior can be seen in part from the entropies of the observed phase transitions, where the Ag (and F respectively) sublattice melts prematurely. (poor ionic conductor) -AgI -AgI (excellent ionic conductor) T = 146 ºC, S = 14.5 J/mol-K -AgI molten AgI S = 11.3 J/mol-K Compare with the an entropy of melting of 24 J/mol-K for NaCl. solid PbF 2 molten PbF 2 S = 16.4 J/mol-K Compare with the an entropy of melting of 35 J/mol-K for MgF 2
Chem Solid State Chemistry Ag + Ion Conductors -AgI Stable below 146 ºCStable below 146 ºC Wurtzite Structure (tetrahedral coordination)Wurtzite Structure (tetrahedral coordination) = S/cm – S/cm = S/cm – S/cm -AgI Stable above 146 ºCStable above 146 ºC BCC Arrangement of I -, molten/ disordered Ag +BCC Arrangement of I -, molten/ disordered Ag + ~ 1 S/cm, E A =0.05 eV ~ 1 S/cm, E A =0.05 eV Conductivity decreases on meltingConductivity decreases on melting RbAg 4 I 5 Highest known conductivity at room temperatureHighest known conductivity at room temperature BCC Arrangement of I -, molten/disordered Ag +BCC Arrangement of I -, molten/disordered Ag + ~ 0.25 S/cm (25 ºC), E A =0.07 eV ~ 0.25 S/cm (25 ºC), E A =0.07 eV
Chem Solid State Chemistry Na + Ion Conductors NaAl 7 O 11 (Na 2 O. nAl 2 O 3 ) FCC like packing of oxygenFCC like packing of oxygen Every fifth layer ¾ of the O 2- ions are missing, Na + ions present. These layers are sandwiched between spinel blocks.Every fifth layer ¾ of the O 2- ions are missing, Na + ions present. These layers are sandwiched between spinel blocks. 2D ionic conductor2D ionic conductor Na 3 Zr 2 PSi 2 O 12 (NASICON) Framework of corner sharing ZrO 6 octhahedra and PO 4 /SiO 4 tetrahedraFramework of corner sharing ZrO 6 octhahedra and PO 4 /SiO 4 tetrahedra Na + ions occupy trigonal prismatic and octahedral sites, ¼ of the Na + sites are emptyNa + ions occupy trigonal prismatic and octahedral sites, ¼ of the Na + sites are empty E A ~ 0.3 eVE A ~ 0.3 eV